#------------------------------------------------------------------------------
#$Date: 2025-11-29 21:38:25 +0100 (Sat 29 de Nov de 2025) $
#$Revision: 303766 $
#$URL: svn://www.crystallography.net/cod/cif/7/71/94/7719430.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7719430
loop_
_publ_author_name
'Ridley, Christopher J.'
'Abdeldaim, Aly H.'
'Bull, Craig L.'
'Tustain, Katherine'
'Clark, Lucy'
_publ_section_title
;
 Pressure-induced tuning of the triangular-honeycomb structure of
 ferroelectric quantum spin liquid candidate, TbInO₃.
;
_journal_issue                   42
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15696
_journal_page_last               15700
_journal_paper_doi               10.1039/d5dt01863c
_journal_volume                  54
_journal_year                    2025
_chemical_formula_moiety         'In O3 Tb'
_chemical_formula_structural     'In O3 Tb'
_chemical_formula_sum            'In O3 Tb'
_chemical_formula_weight         321.747
_chemical_name_common            'Terbium indium oxide'
_space_group_crystal_system      hexagonal
_space_group_IT_number           185
_space_group_name_Hall           'P 6c -2'
_space_group_name_H-M_alt        'P 63 c m'
_symmetry_space_group_name_H-M   'P 63 c m'
_audit_update_record
;
2025-07-19 deposited with the CCDC.	2025-09-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   6.31718(16)
_cell_length_b                   6.31718(16)
_cell_length_c                   12.3065(6)
_cell_measurement_pressure       0.14391
_cell_measurement_temperature    293.00000
_cell_volume                     425.32(3)
_diffrn_ambient_temperature      293.00000
_diffrn_detector                 'ZnS scintillator'
_diffrn_detector_type            custom
_diffrn_measurement_device_type  'PEARL diffractometer'
_diffrn_radiation_monochromator  none
_diffrn_radiation_type           Neutron
_diffrn_source                   'Pulsed neutron source'
_diffrn_source_target            W
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details
;
Calculated using MANTID routines.
;
_exptl_crystal_density_diffrn    7.536980
_pd_instr_dist_spec/detc         800
_pd_instr_dist_src/spec          12800
_pd_instr_location               'SNS, Oak Ridge National Lab'
_pd_meas_2theta_fixed            90
_pd_meas_scan_method
;
Time-of-flight
;
_pd_proc_info_data_reduction
;
Data reduction performed using Mantid
;
_pd_proc_info_excluded_regions
;
?
;
_pd_proc_ls_background_function  'Chebychev polynomial'
_pd_proc_ls_pref_orient_corr
;
No requirement for preferred orientation correction
;
_pd_proc_ls_prof_R_factor        2.94846
_pd_proc_ls_prof_wR_expected     2.76000
_pd_proc_ls_prof_wR_factor       3.51104
_pd_spec_mounting                'TiZr Capsule'
_pd_spec_mount_mode              transmission
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.27211
_refine_ls_matrix_type           sparse
_refine_ls_number_parameters     43
_refine_ls_R_I_factor            1.77761
_refine_ls_shift/su_max          0.0073
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            d5dt01863c1.cif
_cod_data_source_block           p2
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_space_group_crystal_system' value 'Hexagonal' was changed
to 'hexagonal' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 

 Adding full bibliography for 7719421--7719440.cif.
;
_cod_original_cell_volume        425.31(3)
_cod_original_formula_sum        'In O3 Tb '
_cod_database_code               7719430
_pr_proc_ls_profile_function
;
Voigt function convoluted with a back-to-back double exponential.
;
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z '
'-x, -y, z+1/2 '
'-x+y, -x, z '
'-x+y, y, z+1/2 '
'-y, -x, z+1/2 '
'-y, x-y, z '
'y, -x+y, z+1/2 '
'y, x, z '
'x-y, -y, z '
'x-y, x, z+1/2 '
'-x, -x+y, z '
'x, x-y, z+1/2 '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Tb1 Tb 2 0 0 0.260(2) 1 0.1
Tb2 Tb 4 0.3333333 0.6666667 0.2313(18) 1 0.1
In1 In 6 0.340(4) 0 0 1 0.1176497
O1 O 6 0.3090(18) 0 0.1656(13) 1 0.3151487
O2 O 6 0.649(2) 0 0.3241(13) 1 0.3151487
O3 O 2 0 0 0.465(2) 1 0.3151487
O4 O 4 0.3333333 0.6666667 0.0164(17) 1 0.3151487
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
O1 Tb1 O1 96.3(9) 1_555 1_555 6_555
O1 Tb1 O1 96.3(9) 3_555 1_555 1_555
O1 Tb1 O1 96.3(9) 3_555 1_555 6_555
O2 Tb1 O1 76.5(3) 6_545 1_555 3_555
O2 Tb1 O1 76.5(3) 6_545 1_555 1_555
O2 Tb1 O1 169.0(13) 6_545 1_555 6_555
O2 Tb1 O2 109.3(7) 1_455 1_555 6_545
O2 Tb1 O1 76.5(3) 1_455 1_555 3_555
O2 Tb1 O1 169.0(13) 1_455 1_555 1_555
O2 Tb1 O1 76.5(3) 1_455 1_555 6_555
O2 Tb1 O2 109.3(7) 3_665 1_555 1_455
O2 Tb1 O2 109.3(7) 3_665 1_555 6_545
O2 Tb1 O1 169.0(13) 3_665 1_555 3_555
O2 Tb1 O1 76.5(3) 3_665 1_555 1_555
O2 Tb1 O1 76.5(3) 3_665 1_555 6_555
O3 Tb1 O2 70.3(7) 1_555 1_555 3_665
O3 Tb1 O2 70.3(7) 1_555 1_555 1_455
O3 Tb1 O2 70.3(7) 1_555 1_555 6_545
O3 Tb1 O1 120.7(7) 1_555 1_555 3_555
O3 Tb1 O1 120.7(7) 1_555 1_555 1_555
O3 Tb1 O1 120.7(7) 1_555 1_555 6_555
O1 Tb2 O1 108.6(6) 1_565 1_555 3_665
O1 Tb2 O1 108.6(6) 6_555 1_555 1_565
O1 Tb2 O1 108.6(6) 6_555 1_555 3_665
O2 Tb2 O1 76.7(4) 6_555 1_555 6_555
O2 Tb2 O1 75.4(5) 6_555 1_555 1_565
O2 Tb2 O1 171.2(11) 6_555 1_555 3_665
O2 Tb2 O2 98.4(8) 3_665 1_555 6_555
O2 Tb2 O1 75.4(5) 3_665 1_555 6_555
O2 Tb2 O1 171.2(11) 3_665 1_555 1_565
O2 Tb2 O1 76.7(4) 3_665 1_555 3_665
O2 Tb2 O2 98.4(8) 1_565 1_555 3_665
O2 Tb2 O2 98.4(8) 1_565 1_555 6_555
O2 Tb2 O1 171.2(11) 1_565 1_555 6_555
O2 Tb2 O1 76.7(4) 1_565 1_555 1_565
O2 Tb2 O1 75.4(5) 1_565 1_555 3_665
O4 Tb2 O2 119.1(6) 1_555 1_555 1_565
O4 Tb2 O2 119.1(6) 1_555 1_555 3_665
O4 Tb2 O2 119.1(6) 1_555 1_555 6_555
O4 Tb2 O1 69.7(6) 1_555 1_555 6_555
O4 Tb2 O1 69.7(6) 1_555 1_555 1_565
O4 Tb2 O1 69.7(6) 1_555 1_555 3_665
O4 In1 O1 87.1(6) 1_545 1_555 1_555
O4 In1 O4 121.1(11) 8_555 1_555 1_545
O4 In1 O1 87.1(6) 8_555 1_555 1_555
O2 In1 O4 94.7(7) 2_654 1_555 8_555
O2 In1 O4 94.7(7) 2_654 1_555 1_545
O2 In1 O1 176.3(14) 2_654 1_555 1_555
O3 In1 O2 80.3(10) 2_554 1_555 2_654
O3 In1 O4 119.5(6) 2_554 1_555 8_555
O3 In1 O4 119.5(6) 2_554 1_555 1_545
O3 In1 O1 96.0(11) 2_554 1_555 1_555
Tb1 O1 In1 126.2(11) 1_555 1_555 1_555
Tb2 O1 Tb1 105.6(7) 1_545 1_555 1_555
Tb2 O1 In1 107.2(7) 1_545 1_555 1_555
Tb2 O1 Tb2 102.9(7) 8_555 1_555 1_545
Tb2 O1 Tb1 105.6(7) 8_555 1_555 1_555
Tb2 O1 In1 107.2(7) 8_555 1_555 1_555
O4 O1 Tb2 60.3(6) 8_555 1_555 8_555
O4 O1 Tb2 120.3(5) 8_555 1_555 1_545
O4 O1 Tb1 133.7(4) 8_555 1_555 1_555
O4 O1 In1 47.1(5) 8_555 1_555 1_555
O4 O1 O4 79.4(6) 1_545 1_555 8_555
O4 O1 Tb2 120.3(5) 1_545 1_555 8_555
O4 O1 Tb2 60.3(6) 1_545 1_555 1_545
O4 O1 Tb1 133.7(4) 1_545 1_555 1_555
O4 O1 In1 47.1(5) 1_545 1_555 1_555
O2 O1 O4 97.7(4) 6_545 1_555 1_545
O2 O1 O4 172.2(5) 6_545 1_555 8_555
O2 O1 Tb2 116.1(8) 6_545 1_555 8_555
O2 O1 Tb2 52.6(4) 6_545 1_555 1_545
O2 O1 Tb1 53.0(5) 6_545 1_555 1_555
O2 O1 In1 134.9(4) 6_545 1_555 1_555
O2 O1 O2 84.1(7) 3_665 1_555 6_545
O2 O1 O4 172.2(5) 3_665 1_555 1_545
O2 O1 O4 97.7(4) 3_665 1_555 8_555
O2 O1 Tb2 52.6(4) 3_665 1_555 8_555
O2 O1 Tb2 116.1(8) 3_665 1_555 1_545
O2 O1 Tb1 53.0(5) 3_665 1_555 1_555
O2 O1 In1 134.9(4) 3_665 1_555 1_555
O2 O1 O2 76.2(5) 1_555 1_555 3_665
O2 O1 O2 76.2(5) 1_555 1_555 6_545
O2 O1 O4 96.8(5) 1_555 1_555 1_545
O2 O1 O4 96.8(5) 1_555 1_555 8_555
O2 O1 Tb2 52.0(4) 1_555 1_555 8_555
O2 O1 Tb2 52.0(4) 1_555 1_555 1_545
O2 O1 Tb1 107.1(9) 1_555 1_555 1_555
O2 O1 In1 126.7(9) 1_555 1_555 1_555
O3 O1 O2 170.5(7) 2_554 1_555 1_555
O3 O1 O2 110.6(4) 2_554 1_555 3_665
O3 O1 O2 110.6(4) 2_554 1_555 6_545
O3 O1 O4 75.9(5) 2_554 1_555 1_545
O3 O1 O4 75.9(5) 2_554 1_555 8_555
O3 O1 Tb2 126.4(5) 2_554 1_555 8_555
O3 O1 Tb2 126.4(5) 2_554 1_555 1_545
O3 O1 Tb1 82.4(7) 2_554 1_555 1_555
O3 O1 In1 43.8(8) 2_554 1_555 1_555
Tb2 O2 In1 119.9(7) 8_555 1_555 2_655
Tb2 O2 Tb2 101.8(9) 1_545 1_555 8_555
Tb2 O2 In1 119.9(7) 1_545 1_555 2_655
Tb1 O2 Tb2 102.4(6) 1_655 1_555 1_545
Tb1 O2 Tb2 102.4(6) 1_655 1_555 8_555
Tb1 O2 In1 107.9(11) 1_655 1_555 2_655
O3 O2 Tb1 57.7(8) 1_655 1_555 1_655
O3 O2 Tb2 128.0(4) 1_655 1_555 1_545
O3 O2 Tb2 128.0(4) 1_655 1_555 8_555
O3 O2 In1 50.3(8) 1_655 1_555 2_655
O1 O2 O3 94.5(6) 6_655 1_555 1_655
O1 O2 Tb1 50.4(5) 6_655 1_555 1_655
O1 O2 Tb2 107.5(8) 6_655 1_555 1_545
O1 O2 Tb2 52.0(4) 6_655 1_555 8_555
O1 O2 In1 131.9(6) 6_655 1_555 2_655
O1 O2 O1 72.4(6) 3_655 1_555 6_655
O1 O2 O3 94.5(6) 3_655 1_555 1_655
O1 O2 Tb1 50.4(5) 3_655 1_555 1_655
O1 O2 Tb2 52.0(4) 3_655 1_555 1_545
O1 O2 Tb2 107.5(8) 3_655 1_555 8_555
O1 O2 In1 131.9(6) 3_655 1_555 2_655
O1 O2 O1 82.1(6) 1_555 1_555 3_655
O1 O2 O1 82.1(6) 1_555 1_555 6_655
O1 O2 O3 175.8(8) 1_555 1_555 1_655
O1 O2 Tb1 118.1(9) 1_555 1_555 1_655
O1 O2 Tb2 51.4(4) 1_555 1_555 1_545
O1 O2 Tb2 51.4(4) 1_555 1_555 8_555
O1 O2 In1 134.0(9) 1_555 1_555 2_655
O4 O2 O1 106.5(5) 4_545 1_555 1_555
O4 O2 O1 107.5(3) 4_545 1_555 3_655
O4 O2 O1 171.3(6) 4_545 1_555 6_655
O4 O2 O3 76.9(5) 4_545 1_555 1_655
O4 O2 Tb1 122.6(6) 4_545 1_555 1_655
O4 O2 Tb2 78.1(6) 4_545 1_555 1_545
O4 O2 Tb2 134.2(6) 4_545 1_555 8_555
O4 O2 In1 41.8(4) 4_545 1_555 2_655
O4 O2 O4 71.2(5) 2_665 1_555 4_545
O4 O2 O1 106.5(5) 2_665 1_555 1_555
O4 O2 O1 171.3(6) 2_665 1_555 3_655
O4 O2 O1 107.5(3) 2_665 1_555 6_655
O4 O2 O3 76.9(5) 2_665 1_555 1_655
O4 O2 Tb1 122.6(6) 2_665 1_555 1_655
O4 O2 Tb2 134.2(6) 2_665 1_555 1_545
O4 O2 Tb2 78.1(6) 2_665 1_555 8_555
O4 O2 In1 41.8(4) 2_665 1_555 2_655
In1 O3 In1 116.1(4) 2_555 1_555 5_555
In1 O3 In1 116.1(4) 10_555 1_555 2_555
In1 O3 In1 116.1(4) 10_555 1_555 5_555
Tb1 O3 In1 101.5(8) 1_555 1_555 10_555
Tb1 O3 In1 101.5(8) 1_555 1_555 2_555
Tb1 O3 In1 101.5(8) 1_555 1_555 5_555
O2 O3 Tb1 52.0(6) 3_665 1_555 1_555
O2 O3 In1 49.5(5) 3_665 1_555 10_555
O2 O3 In1 120.6(6) 3_665 1_555 2_555
O2 O3 In1 120.6(6) 3_665 1_555 5_555
O2 O3 O2 86.1(8) 6_545 1_555 3_665
O2 O3 Tb1 52.0(6) 6_545 1_555 1_555
O2 O3 In1 120.6(6) 6_545 1_555 10_555
O2 O3 In1 120.6(6) 6_545 1_555 2_555
O2 O3 In1 49.5(5) 6_545 1_555 5_555
O2 O3 O2 86.1(8) 1_455 1_555 6_545
O2 O3 O2 86.1(8) 1_455 1_555 3_665
O2 O3 Tb1 52.0(6) 1_455 1_555 1_555
O2 O3 In1 120.6(6) 1_455 1_555 10_555
O2 O3 In1 49.5(5) 1_455 1_555 2_555
O2 O3 In1 120.6(6) 1_455 1_555 5_555
O1 O3 O2 136.7(3) 5_555 1_555 1_455
O1 O3 O2 89.7(4) 5_555 1_555 6_545
O1 O3 O2 136.7(3) 5_555 1_555 3_665
O1 O3 Tb1 141.7(4) 5_555 1_555 1_555
O1 O3 In1 98.5(8) 5_555 1_555 10_555
O1 O3 In1 98.5(8) 5_555 1_555 2_555
O1 O3 In1 40.2(5) 5_555 1_555 5_555
O1 O3 O1 64.9(7) 2_555 1_555 5_555
O1 O3 O2 89.7(4) 2_555 1_555 1_455
O1 O3 O2 136.7(3) 2_555 1_555 6_545
O1 O3 O2 136.7(3) 2_555 1_555 3_665
O1 O3 Tb1 141.7(4) 2_555 1_555 1_555
O1 O3 In1 98.5(8) 2_555 1_555 10_555
O1 O3 In1 40.2(5) 2_555 1_555 2_555
O1 O3 In1 98.5(8) 2_555 1_555 5_555
O1 O3 O1 64.9(7) 10_555 1_555 2_555
O1 O3 O1 64.9(7) 10_555 1_555 5_555
O1 O3 O2 136.7(3) 10_555 1_555 1_455
O1 O3 O2 136.7(3) 10_555 1_555 6_545
O1 O3 O2 89.7(4) 10_555 1_555 3_665
O1 O3 Tb1 141.7(4) 10_555 1_555 1_555
O1 O3 In1 40.2(5) 10_555 1_555 10_555
O1 O3 In1 98.5(8) 10_555 1_555 2_555
O1 O3 In1 98.5(8) 10_555 1_555 5_555
In1 O4 In1 119.1(2) 1_565 1_555 3_665
In1 O4 In1 119.1(2) 6_555 1_555 1_565
In1 O4 In1 119.1(2) 6_555 1_555 3_665
Tb2 O4 In1 95.5(6) 1_555 1_555 6_555
Tb2 O4 In1 95.5(6) 1_555 1_555 1_565
Tb2 O4 In1 95.5(6) 1_555 1_555 3_665
O1 O4 Tb2 50.0(4) 6_555 1_555 1_555
O1 O4 In1 45.7(4) 6_555 1_555 6_555
O1 O4 In1 119.6(7) 6_555 1_555 1_565
O1 O4 In1 113.0(6) 6_555 1_555 3_665
O1 O4 O1 83.1(6) 1_565 1_555 6_555
O1 O4 Tb2 50.0(4) 1_565 1_555 1_555
O1 O4 In1 113.0(6) 1_565 1_555 6_555
O1 O4 In1 45.7(4) 1_565 1_555 1_565
O1 O4 In1 119.6(7) 1_565 1_555 3_665
O1 O4 O1 83.1(6) 3_665 1_555 1_565
O1 O4 O1 83.1(6) 3_665 1_555 6_555
O1 O4 Tb2 50.0(4) 3_665 1_555 1_555
O1 O4 In1 119.6(7) 3_665 1_555 6_555
O1 O4 In1 113.0(6) 3_665 1_555 1_565
O1 O4 In1 45.7(4) 3_665 1_555 3_665
O2 O4 O1 89.2(3) 10_554 1_555 3_665
O2 O4 O1 141.4(3) 10_554 1_555 1_565
O2 O4 O1 133.5(3) 10_554 1_555 6_555
O2 O4 Tb2 139.1(3) 10_554 1_555 1_555
O2 O4 In1 103.7(7) 10_554 1_555 6_555
O2 O4 In1 105.6(7) 10_554 1_555 1_565
O2 O4 In1 43.5(4) 10_554 1_555 3_665
O2 O4 O2 69.1(5) 2_664 1_555 10_554
O2 O4 O1 133.5(3) 2_664 1_555 3_665
O2 O4 O1 89.2(3) 2_664 1_555 1_565
O2 O4 O1 141.4(3) 2_664 1_555 6_555
O2 O4 Tb2 139.1(3) 2_664 1_555 1_555
O2 O4 In1 105.6(7) 2_664 1_555 6_555
O2 O4 In1 43.5(4) 2_664 1_555 1_565
O2 O4 In1 103.7(7) 2_664 1_555 3_665
O2 O4 O2 69.1(5) 5_564 1_555 2_664
O2 O4 O2 69.1(5) 5_564 1_555 10_554
O2 O4 O1 141.4(3) 5_564 1_555 3_665
O2 O4 O1 133.5(3) 5_564 1_555 1_565
O2 O4 O1 89.2(3) 5_564 1_555 6_555
O2 O4 Tb2 139.1(3) 5_564 1_555 1_555
O2 O4 In1 43.5(4) 5_564 1_555 6_555
O2 O4 In1 103.7(7) 5_564 1_555 1_565
O2 O4 In1 105.6(7) 5_564 1_555 3_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Tb1 O1 2.270(19) 1_555 6_555
Tb1 O1 2.270(19) 1_555 1_555
Tb1 O1 2.270(19) 1_555 3_555
Tb1 O2 2.352(17) 1_555 6_545
Tb1 O2 2.352(17) 1_555 1_455
Tb1 O2 2.352(17) 1_555 3_665
Tb1 O3 2.52(4) 1_555 1_555
Tb2 O1 2.331(11) 1_555 3_665
Tb2 O1 2.331(11) 1_555 1_565
Tb2 O1 2.331(11) 1_555 6_555
Tb2 O2 2.350(14) 1_555 6_555
Tb2 O2 2.350(14) 1_555 3_665
Tb2 O2 2.350(14) 1_555 1_565
Tb2 O4 2.64(3) 1_555 1_555
In1 O1 2.047(16) 1_555 1_555
In1 O4 2.095(11) 1_555 1_545
In1 O4 2.095(11) 1_555 8_555
In1 O2 2.166(16) 1_555 2_654
In1 O3 2.19(2) 1_555 2_554
O1 In1 2.047(16) 1_555 1_555
O1 Tb1 2.270(19) 1_555 1_555
O1 Tb2 2.331(11) 1_555 1_545
O1 Tb2 2.331(11) 1_555 8_555
O1 O4 2.855(17) 1_555 8_555
O1 O4 2.855(17) 1_555 1_545
O1 O2 2.863(17) 1_555 6_545
O1 O2 2.863(17) 1_555 3_665
O1 O2 2.90(2) 1_555 1_555
O1 O3 3.15(3) 1_555 2_554
O2 In1 2.166(16) 1_555 2_655
O2 Tb2 2.350(14) 1_555 8_555
O2 Tb2 2.350(14) 1_555 1_545
O2 Tb1 2.352(17) 1_555 1_655
O2 O3 2.81(2) 1_555 1_655
O2 O1 2.863(17) 1_555 6_655
O2 O1 2.863(17) 1_555 3_655
O2 O1 2.90(2) 1_555 1_555
O2 O4 3.13(2) 1_555 4_545
O2 O4 3.13(2) 1_555 2_665
O3 In1 2.19(2) 1_555 5_555
O3 In1 2.19(2) 1_555 2_555
O3 In1 2.19(2) 1_555 10_555
O3 Tb1 2.52(4) 1_555 1_555
O3 O2 2.81(2) 1_555 3_665
O3 O2 2.81(2) 1_555 6_545
O3 O2 2.81(2) 1_555 1_455
O3 O1 3.15(3) 1_555 5_555
O3 O1 3.15(3) 1_555 2_555
O3 O1 3.15(3) 1_555 10_555
O4 In1 2.095(11) 1_555 3_665
O4 In1 2.095(11) 1_555 1_565
O4 In1 2.095(11) 1_555 6_555
O4 Tb2 2.64(3) 1_555 1_555
O4 O1 2.855(17) 1_555 6_555
O4 O1 2.855(17) 1_555 1_565
O4 O1 2.855(17) 1_555 3_665
O4 O2 3.13(2) 1_555 10_554
O4 O2 3.13(2) 1_555 2_664
O4 O2 3.13(2) 1_555 5_564
